- Nano Express
- Open Access
Functional Application of Noble Metal Nanoparticles In Situ Synthesized on Ramie Fibers
© Tang et al. 2015
- Received: 19 August 2015
- Accepted: 8 September 2015
- Published: 17 September 2015
Different functions were imparted to ramie fibers through treatment with noble metal nanoparticles including silver and gold nanoparticles. The in situ synthesis of silver and gold nanoparticles was achieved by heating in the presence of ramie fibers in the corresponding solutions of precursors. The unique optical property of synthesized noble metal nanoparticles, i.e., localized surface plasmon resonance, endowed ramie fibers with bright colors. Color strength (K/S) of fibers increased with heating temperature. Silver nanoparticles were obtained in alkaline solution, while acidic condition was conducive to gold nanoparticles. The optical properties of treated ramie fibers were investigated using UV-vis absorption spectroscopy. Scanning electron microscopy (SEM) was employed to observe the morphologies of silver and gold nanoparticles in situ synthesized on fibers. The ramie fibers treated with noble metal nanoparticles showed remarkable catalytic activity for reduction of 4-nitrophenol (4-NP) by sodium borohydride. Moreover, the silver nanoparticle treatment showed significant antibacterial property on ramie fibers.
- Silver nanoparticle
- Gold nanoparticle
- In situ synthesis
Functionalization of textiles with nanoparticles has attracted intensive attentions of scientists and engineers in recent years. A number of strategies have been developed to enhance functions of textiles [1–4], such as antibacterial treatment [1, 5], self-cleaning coating [6, 7], and UV protection enhancement [8, 9]. Semiconductor (e.g., TiO2 and ZnO) nanoparticles have been applied to textiles for functions such as UV-blocking and self-cleaning [10, 11]. Silver nanoparticle as a broad antibacterial agent is widely used for antibacterial finishing of textiles [12, 13]. Besides antibacterial property, noble metal nanoparticles (e.g., silver and gold) possess particular localized surface plasmon resonance (LSPR) property, which leads to bright colors. Some strategies have been developed to utilize noble metal nanoparticles to functionalize different fibers such as cotton, wool, and silk. The coloration of fibers has been achieved through treatment with silver nanoparticles, taking advantage of the LSPR optical property of noble metal nanoparticles [5, 14, 15]. Similarly, gold nanoparticles can also endow fabrics with different functions including colors, UV protection, and antibacterial properties [16–18].
Ramie from a perennial herbaceous plant of the Urticaceae family is one of the most important bast plant fibers and has a silky luster. It is superior to cotton and silk in length and strength [19–21]. Ramie fibers have been applied to an increasing number of textile products including canvas, clothing fabrics, towels, cordages, and garments, due to their high tenacity, excellent thermal conductivity, good comfort, and significant tensile properties [21–23]. China and several other Asian countries are main producing areas of ramie fiber [24, 25]. Functional modification of ramie fibers is one way to promote product value and satisfy the increasing needs from consumers. Regarding modifications of ramie, Zheng et al. coated ramie fabrics with titanium dioxide (TiO2) nanoparticles via a dip-pad-dry process . The ramie fabrics treated with TiO2 showed antibacterial and UV-protective properties. However, the research focused on the functionalization of ramie with nanoparticles is very limited.
In this study, the functionalization of ramie fibers was realized through in situ synthesis of silver and gold nanoparticles. The silver nanoparticle-treated ramie fiber displayed a yellow color, while gold nanoparticles endowed the ramie fiber with red and purple colors. The changes in color strength (K/S) of ramie fibers with pH value of solution were also observed. Antibacterial property of the ramie fibers treated with silver nanoparticles was evaluated. The color fastness to washing of the treated ramie was tested. Moreover, the catalytic ability of ramie fibers treated with silver and gold nanoparticles was determined using reduction of 4-nitrophenol by sodium borohydride as a model reaction.
AgNO3 (>99 %), tetrachloroauric (III) acid (HAuCl4 · 3H2O, >99 %), NaOH (≥97.0 %), acetic acid (>99.7 %), 4-nitrophenol (≥99 %), and sodium borohydride (>98 %) were purchased from Sigma-Aldrich. All chemicals were analytic grade reagents and used without further purification. Ramie fibers and fabrics were kindly provided by Engineering Research Center for Clean Production of Textile Printing in Wuhan Textile University. They were used without pretreatment.
In Situ Synthesis of Silver and Gold Nanoparticles on Ramie Fibers
Ramie fibers were washed for 3 min with hot water (70 °C) followed by rinsing with deionized water at room temperature. The washed fibers were immersed in precursor solutions of metal nanoparticles (AgNO3 for silver nanoparticles and HAuCl4 for gold nanoparticles) with different concentrations. The weight ratio of aqueous solution to fibers was 80. The ramie fibers were immersed in precursor solutions for 15 min at room temperature and the pH values of the solutions were adjusted. After that, the solutions were heated at different temperatures for 60 min in an oscillating water bath. The treated fibers were rinsed with running deionized water and dried at room temperature. The details of the corresponding experimental conditions for in situ synthesis of silver and gold nanoparticles are listed in Additional file 1: Tables S1 and Additional file 1: S2, respectively.
Color Fastness to Washing
Washing fastness was evaluated in accordance with Australian Standard AS 2001.4.15—2006. The ramie fabrics treated with silver or gold nanoparticles were washed for 45 min at 50 °C in the presence of ECE reference detergent (4 g/L) by using a lab dyeing machine (Ahiba, Top Speed Nuance). The CIE Lab color coordinate values (L*, a*, and b*) for each specimen were measured before and after washing. L* represents the lightness/darkness, a* value represents the red or green chroma, and b* represents the chromaticity coordinate for yellow/blue. The color difference (ΔE) was obtained based on the changes in color coordinates (ΔL*, Δa*, and Δb*) with the formula: ΔE = [(ΔL*)2 + (Δa*)2 + (Δb*)2]1/2. The color difference (ΔE) of ramie fabrics before and after washing was measured by spectrophotometer to assess washing fastness of ramie fabrics according to Australian Standard AS 2001.4.A05—2004.
To investigate the catalytic efficiency and reusability of the ramie fibers treated with noble metal nanoparticles, the catalytic conversion of 4-nitrophenol into 4-aminophenol by sodium borohydride (NaBH4) was performed in the presence of untreated and treated ramie. In a typical experiment, 1.0 mL of NaBH4 solution (3.42 M) was added into 40 mL of 4-nitrophenol aqueous solution (0.025 mM). Subsequently, 0.0485 g of untreated ramie fibers or treated ramie fibers (Ag-90-10-1, Ag-90-10-3 and Au-90-5-6) was added into the mixing solution of 4-nitrophenol and NaBH4 under vigorous stirring. UV–visible absorption spectra were monitored during the conversion of 4-nitrophenol into 4-aminophenol.
Antibacterial Test Against Gram-Negative Bacteria
Gram-negative bacteria, Escherichia coli (E. coli) (ATCC 11229), were used as test organisms. Antibacterial test was performed on untreated and silver nanoparticle-treated ramie fibers. The antibacterial test was carried out according to the AATCC 100-2004 (Clause 10.2) test standard with slight modifications. Fifty microliters of bacteria were added to treated samples in separate flasks. After 1.0 min, 50 mL of sterile deionized water was poured into each flask, followed by vigorous shaking. Then, the flasks were incubated for 18 h in a shaker oven at 120 rpm and 37 °C. After that, the fiber samples were collected and the solution left in the flask was further diluted to get countable number of bacterial colonies. A 103 dilution was suitable for obtaining colonies between 30 and 300. One hundred microliters of the 103 dilution obtained was placed on the nutrient agar plates. These plates were then incubated for 18 h in an oven at 37 °C. The bacterial activity was recorded by photography. The test was carried out in triplicate and the entire experiments were repeated three times.
Heating may promote the in situ synthesis of noble metal nanoparticles in the presence of ramie fibers. To investigate the influence of heating on synthesis of noble metal nanoparticles, different temperatures were tested when other reaction conditions remained unchanged. Additional file 1: Tables S3 and S4 displays the detailed conditions for synthesis of silver and gold nanoparticles. Additional file 1: Figure S2a shows the K/S curves of ramie fibers treated with silver nanoparticles obtained at different temperatures. The result reveals that the silver nanoparticles can be obtained in situ on ramie fibers at a low temperature (40 °C). The K/S value increased as the reaction temperature increased (Additional file 1: Figure S2b). It is found that high temperature led to high color strength (K/S) of ramie fibers. The gold nanoparticles were also prepared on ramie fibers at 40 °C (Additional file 1: Figure S3a). The K/S value increased when the temperature was increased to 70 from 40 °C. Nevertheless, the maximum K/S value changed slightly when the reaction temperature was between 70 ~ 90 °C (Additional file 1: Figure S3b), implying that nearly all the gold ions were reduced at 70 °C. The trend of change in K/S curves of gold nanoparticle-treated ramie fibers was different from that of silver nanoparticle-treated ramie fibers, which may be due to difference in redox potential of silver and gold.
Content of silver in different ramie fibers treated with silver nanoparticles
Content of Ag (wt%)
Content of Ag (wt%)
Content of gold in different ramie fibers treated with gold nanoparticles
Content of Au (wt%)
Content of Au (wt%)
Color fastness of dyed fabrics is important in practical applications. The same as ramie fibers, the ramie fabrics were colored by in situ synthesized silver and gold nanoparticles. The color fastness to washing of the ramie fabrics treated with noble metal nanoparticles was evaluated. The ramie fabrics were washed for 45 min in the presence of ECE reference detergent at 50 °C under each washing cycle. The color differences (ΔE) of the ramie fabrics before and after washing are shown in Additional file 1: Figure S5. The visible color difference of silver nanoparticle-treated ramie fabrics after the first washing cycle was found with ΔE of 5.2 (Additional file 1: Figure S5). However, the average ΔE value of fabrics treated with silver nanoparticles did not increased notably with further increase in number of washing cycles. Compared with silver nanoparticle-treated ramie fabrics, the gold nanoparticle-treated ramie fabrics showed very good washing color fastness. The average ΔE value of fabrics treated with gold nanoparticles was 2.0 after first washing cycle (Additional file 1: Figure S5), which corresponds to the gray scale rating of 4. The color difference of gold nanoparticle-treated fabrics changed slightly and remained stable as the number of washing cycles increased, which indicates that the ramie fabrics colored by in situ synthesized gold nanoparticles exhibited good washing color fastness.
In addition to silver nanoparticle-treated ramie, catalysis ability of the fibers treated with gold nanoparticles was investigated as well. The absorption peak at 400 nm of 4-nitrophenol decreased gradually in the presence of gold nanoparticle-treated ramie fibers (Au-90-5-6) with reaction time (Additional file 1: Figure S6a). The plot of peak intensity at 400 nm versus time proves that the ramie fibers with gold nanoparticles exhibit evident catalytic activity (Additional file 1: Figure S6b). The results indicate that the ramie fibers with noble metal (silver and gold) nanoparticles show effective catalysis cavity.
Silver nanoparticles as antibacterial agents have been used widely for antibacterial finishing of textile products [12, 37]. In the present study, the antibacterial properties of silver nanoparticle-treated ramie fibers were evaluated against the Gram-negative bacteria, E. coli. Additional file 1: Figure S7 shows the photographs of the bacterial colonies on blank (control) sample, untreated ramie fibers, silver nanoparticle-treated fibers (Ag-90-10-3). Plenty of colonies of viable bacteria were seen on agar plates corresponding to the control sample and untreated fibers (Additional file 1: Figure S7a, b). Whereas, no bacteria colonies were found on agar plates of ramie fibers treated with silver nanoparticles (Additional file 1: Figure S7c), revealing that the silver nanoparticles on fibers inhibited the growth of bacteria. Therefore, it is suggested that the in situ synthesized silver nanoparticles endow ramie fiber with strong antibacterial property, which enhances the function of ramie fibers.
Additional file 1: Figure S8 displays the 13C solid-state NMR spectra of ramie fibers before and after treatment with noble metal nanoparticles. It is well-known that the NMR technique probes the signal from the overall sample volume and the NMR intensity is proportional to the number of spins. Therefore, for the present ramie samples, the NMR spectra provide us the structure and dynamics information of the bulk molecules rather than the surface because of its small surface-to-volume ratio. The NMR spectra corresponding to untreated and treated ramie fibers were nearly identical, which indicates that the in situ synthesis of noble metal nanoparticles did not change visibly the chemical structures of the bulk ramie. As an indispensable compensation to NMR, FTIR detects the structure and dynamics of the surface molecules. To understand the surface structure change of the treated ramie fibers, FTIR measurements were performed for all the three samples. Comparing with the FTIR spectrum of untreated ramie (Curve a in Additional file 1: Figure S9), no obvious differences were found in the FTIR spectra of the fabrics after treatment with silver and gold nanoparticles (Curves b and c in Additional file 1: Figure S9). These results suggest that there is no evidence of degradation on the surface of ramie fibers. The main chemical structures of the surface of ramie fibers kept essentially unchanged during the in situ synthesis of silver and gold nanoparticles, which is consistent with the cases of cotton and bamboo treated with noble metal nanoparticles [16, 38]. The ramie is composed mainly of cellulose [39–41]. Cellulose as a reducing agent has been used for synthesis of silver and gold particles because of the presence of hydroxyl groups . Additionally, other components of ramie including lignin, gum, and pectin may reduce silver or gold ions to form nanoparticles, due to their reducibility [43–45]. Further investigation on the mechanism for the reduction of silver and gold ions by ramie is in progress.
Silver and gold nanoparticles were in situ synthesized on ramie fibers at different pH values through heating. Alkaline condition is required to synthesize silver nanoparticle in the presence of ramie. Whereas, acidic condition facilitated the synthesis of gold nanoparticles on ramie fibers. The formation of silver and gold nanoparticle imparted bright colors to ramie fibers. The color strength (K/S) of ramie fibers increased with concentration of precursor ions in solution. UV-vis reflectance absorption spectroscopy and SEM demonstrated that silver and gold nanoparticles were produced on ramie fibers. The contents of silver or gold were analyzed under different conditions. Significantly, the ramie fibers treated with in situ synthesized silver and gold nanoparticles showed remarkable catalytic activity for reduction of 4-nitrophenol. The treated ramie fibers could be separated readily and reused in catalyzed reaction. The ramie fabrics treated with gold nanoparticle had good color fastness to washing. Additionally, the silver nanoparticle-treated fibers showed significant antibacterial property. The finishing of ramie fibers based on the in situ synthesis of noble metal nanoparticles would pave the way for the development of functional ramie fibers.
This research was supported by the National Natural Science Foundation of China (NSFC 51273153 and 51403162).
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Wang Q, Fan X, Hu Y, Yuan J, Cui L, Wang P. Antibacterial functionalization of wool fabric via immobilizing lysozymes. Bioprocess Biosyst Eng. 2009;32:633–9.View ArticleGoogle Scholar
- Milosevic M, Radoicic M, Saponjic Z, Nunney T, Deeks C, Lazic V, et al. In situ photoreduction of Ag+-ions by TiO2 nanoparticles deposited on cotton and cotton/PET fabrics. Cellulose. 2014;21:3781–95.View ArticleGoogle Scholar
- Mahltig B, Haufe H, Bottcher H. Functionalisation of textiles by inorganic sol-gel coatings. J Mater Chem. 2005;15:4385–98.View ArticleGoogle Scholar
- Zemljic LF, Volmajer J, Ristic T, Bracic M, Sauperl O, Kreze T. Antimicrobial and antioxidant functionalization of viscose fabric using chitosan-curcumin formulations. Text Res J. 2014;84:819–30.View ArticleGoogle Scholar
- Tang B, Li J, Hou X, Afrin T, Sun L, Wang X. Colorful and antibacterial silk fiber from anisotropic silver nanoparticles. Ind Eng Chem Res. 2013;52:4556–63.View ArticleGoogle Scholar
- Bozzi A, Yuranova T, Guasaquillo I, Laub D, Kiwi J. Self-cleaning of modified cotton textiles by TiO2 at low temperatures under daylight irradiation. J Photoch Photobio A. 2005;174:156–64.View ArticleGoogle Scholar
- Abidi N, Cabrales L, Hequet E. Functionalization of a cotton fabric surface with titania nanosols: applications for self-cleaning and UV-protection properties. ACS Appl Mat Interfaces. 2009;1:2141–6.View ArticleGoogle Scholar
- Gorjanc M, Jazbec K, Sala M, Zaplotnik R, Vesel A, Mozetic M. Creating cellulose fibres with excellent UV protective properties using moist CF4 plasma and ZnO nanoparticles. Cellulose. 2014;21:3007–21.View ArticleGoogle Scholar
- Shen Y, Zhen L, Huang D, Xue J. Improving anti-UV performances of cotton fabrics via graft modification using a reactive UV-absorber. Cellulose. 2014;21:3745–54.View ArticleGoogle Scholar
- Radetic M. Functionalization of textile materials with TiO2 nanoparticles. J Photoch Photobio C. 2013;16:62–76.View ArticleGoogle Scholar
- Broasca G, Borcia G, Dumitrascu N, Vrinceanu N. Characterization of ZnO coated polyester fabrics for UV protection. Appl Surf Sci. 2013;279:272–8.View ArticleGoogle Scholar
- Dastjerdi R, Montazer M. A review on the application of inorganic nano-structured materials in the modification of textiles: focus on anti-microbial properties. Colloid Surface B. 2010;79:5–18.View ArticleGoogle Scholar
- Lee HJ, Yeo SY, Jeong SH. Antibacterial effect of nanosized silver colloidal solution on textile fabrics. J Mater Sci. 2003;38:2199–204.View ArticleGoogle Scholar
- Tang B, Wang J, Xu S, Afrin T, Xu W, Sun L, et al. Application of anisotropic silver nanoparticles: multifunctionalization of wool fabric. J Colloid Interface Sci. 2011;356:513–8.View ArticleGoogle Scholar
- Kelly FM, Johnston JH. Colored and functional silver nanoparticle—wool fiber composites. ACS Appl Mat Interfaces. 2011;3:1083–92.View ArticleGoogle Scholar
- Tang B, Sun L, Li J, Kaur J, Zhu H, Qin S, et al. Functionalization of bamboo pulp fabrics with noble metal nanoparticles. Dyes Pigm. 2015;113:289–98.View ArticleGoogle Scholar
- Tang B, Sun L, Kaur J, Yu Y, Wang X. In-situ synthesis of gold nanoparticles for multifunctionalization of silk fabrics. Dyes Pigm. 2014;103:183–90.View ArticleGoogle Scholar
- Tang B, Tao J, Xu S, Wang J, Hurren C, Xu W, et al. Using hydroxy carboxylate to synthesize gold nanoparticles in heating and photochemical reactions and their application in textile colouration. Chem Eng J. 2011;172:601–7.View ArticleGoogle Scholar
- Yi J, Chen J, Liu Z-T, Liu Z-W. Grafting of polystyrene and poly(p-chlorostyrene) from the surface of ramie fiber via RAFT polymerization. J Appl Polym Sci. 2010;117:3551–7.Google Scholar
- Liu Z-T, Yang Y, Zhang L, Sun P, Liu Z-W, Lu J, et al. Study on the performance of ramie fiber modified with ethylenediamine. Carbohydr Polym. 2008;71:18–25.View ArticleGoogle Scholar
- Cengiz TG, Babalık FC. The effects of ramie blended car seat covers on thermal comfort during road trials. Int J Ind Ergon. 2009;39:287–94.View ArticleGoogle Scholar
- Chen J, Yi J, Sun P, Liu Z-T, Liu Z-W. Grafting from ramie fiber with poly(MMA) or poly(MA) via reversible addition-fragmentation chain transfer polymerization. Cellulose. 2009;16:1133–45.View ArticleGoogle Scholar
- Liu X, Chen J, Sun P, Liu Z-W, Liu Z-T. Grafting modification of ramie fibers with poly(2,2,2-trifluoroethyl methacrylate) via reversible addition–fragmentation chain transfer (RAFT) polymerization in supercritical carbon dioxide. React Funct Polym. 2010;70:972–9.View ArticleGoogle Scholar
- Liu F, Liang X, Zhang N, Huang Y, Zhang S. Effect of growth regulators on yield and fiber quality in ramie (Boemheria nivea (L.) Gaud.), China grass. Field Crops Res. 2001;69:41–6.View ArticleGoogle Scholar
- Liu Z-T, Yang Y, Zhang L, Liu Z-W, Xiong H. Study on the cationic modification and dyeing of ramie fiber. Cellulose. 2007;14:337–45.View ArticleGoogle Scholar
- Zheng GH, Ji FL, Ren J. Multifunctional finishing of ramie fabric using titanium dioxide nanoparticles. In: Xiong JQ, editor. Advanced materials and information technology processing II. Zurich-Durnten: Trans Tech; 2012. p. 185–90.Google Scholar
- Kelly KL, Coronado E, Zhao LL, Schatz GC. The optical properties of metal nanoparticles: the influence of size, shape, and dielectric environment. J Phys Chem B. 2003;107:668–77.View ArticleGoogle Scholar
- Velikov KP, Zegers GE, van Blaaderen A. Synthesis and characterization of large colloidal silver particles. Langmuir. 2003;19:1384–9.View ArticleGoogle Scholar
- Thomas S, Nair SK, Jamal EMA, Al-Harthi SH, Varma MR, Anantharaman MR. Size-dependent surface plasmon resonance in silver silica nanocomposites. Nanotechnology. 2008;19:075710.View ArticleGoogle Scholar
- Ghosh SK, Kundu S, Mandal M, Pal T. Silver and gold nanocluster catalyzed reduction of methylene blue by arsine in a micellar medium. Langmuir. 2002;18:8756–60.View ArticleGoogle Scholar
- Herves P, Perez-Lorenzo M, Liz-Marzan LM, Dzubiella J, Lu Y, Ballauff M. Catalysis by metallic nanoparticles in aqueous solution: model reactions. Chem Soc Rev. 2012;41:5577–87.View ArticleGoogle Scholar
- Lee JH, Kang S, Lee JY, Jung JH. A tetrazole-based metallogel induced with Ag+ ion and its silver nanoparticle in catalysis. Soft Matter. 2012;8:6557–63.View ArticleGoogle Scholar
- Cloud JE, Taylor LW, Yang Y. A simple and effective method for controllable synthesis of silver and silver oxide nanocrystals. RSC Adv. 2014;4:24551–9.View ArticleGoogle Scholar
- Liang M, Su R, Huang R, Qi W, Yu Y, Wang L, et al. Facile in situ synthesis of silver nanoparticles on procyanidin-grafted eggshell membrane and their catalytic properties. ACS Appl Mat Interfaces. 2014;6:4638–49.View ArticleGoogle Scholar
- Ashraf S, Saifur R, Sher F, Khalid ZM, Mehmood M, Hussain I. Synthesis of cellulose-metal nanoparticle composites: development and comparison of different protocols. Cellulose. 2014;21:395–405.View ArticleGoogle Scholar
- Jia X, Ma X, Wei D, Dong J, Qian W. Direct formation of silver nanoparticles in cuttlebone-derived organic matrix for catalytic applications. Colloid Surface A. 2008;330:234–40.View ArticleGoogle Scholar
- Chen X, Schluesener HJ. Nanosilver: a nanoproduct in medical application. Toxicol Lett. 2008;176:1–12.View ArticleGoogle Scholar
- Tang B, Kaur J, Sun L, Wang X. Multifunctionalization of cotton through in situ green synthesis of silver nanoparticles. Cellulose. 2013;20:3053–65.View ArticleGoogle Scholar
- Thakur R, Sarkar CR, Sarmah R. Chemical composition of some varieties of ramie and their fibre characteristics. Indian J Fibre Text. 1999;24:276–8.Google Scholar
- Choi HY, Lee JS. Effects of surface treatment of ramie fibers in a ramie/poly(lactic acid) composite. Fibers Polym. 2012;13:217–23.View ArticleGoogle Scholar
- Fan X-S, Liu Z-W, Liu Z-T, Lu J. A novel chemical degumming process for ramie bast fiber. Text Res J. 2010;80:2046–51.View ArticleGoogle Scholar
- Tan J, Liu R, Wang W, Liu W, Tian Y, Wu M, et al. Controllable aggregation and reversible pH sensitivity of AuNPs regulated by carboxymethyl cellulose. Langmuir. 2009;26:2093–8.View ArticleGoogle Scholar
- Coccia F, Tonucci L, Bosco D, Bressan M, d’Alessandro N. One-pot synthesis of lignin-stabilised platinum and palladium nanoparticles and their catalytic behaviour in oxidation and reduction reactions. Green Chem. 2012;14:1073–8.View ArticleGoogle Scholar
- Dhar S, Reddy EM, Shiras A, Pokharkar V, Prasad BLV. Natural gum reduced/stabilized gold nanoparticles for drug delivery formulations. Chem-Eur J. 2008;14:10244–50.View ArticleGoogle Scholar
- Zahran MK, Ahmed HB, El-Rafie MH. Facile size-regulated synthesis of silver nanoparticles using pectin. Carbohydr Polym. 2014;111:971–8.View ArticleGoogle Scholar